Please copy and paste this embed script to where you want to embed

NORSOK STANDARD

CO2 CORROSION RATE CALCULATION MODEL

M-506 Rev. 1, June 1998

This NORSOK standard is developed by NTS with broad industry participation. Please note that whilst every effort has been made to ensure the accuracy of this standard, neither OLF nor TBL or any of their members will assume liability for any use thereof. NTS is responsible for the administration and publication of this standard. Norwegian Technology Standards Institution Oscarsgt. 20, Postbox 7072 Majorstua N-0306 Oslo, NORWAY Telephone: + 47 22 59 67 00 Fax: + 47 22 59 67 29 Email: [email protected] Website: http://www.nts.no/norsok Copyrights reserved

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

CONTENTS FOREWORD INTRODUCTION

2 2

1 SCOPE

3

2 NORMATIVE REFERENCES

3

3 DEFINITIONS AND ABBREVIATIONS 3.1 Definitions 3.2 Symbols

3 3 3

4 PRINCIPLES FOR USE OF THE COMPUTER PROGRAM

4

5 DESCRIPTION OF THE CO2 CORROSION RATE MODEL 5.1 General 5.2 The corrosion model 5.3 The effect of glycol and corrosion inhibitors

5 5 6 7

6 STRUCTURE OF THE COMPUTER PROGRAMME

8

7 INPUT PARAMETERS 7.1 Basic input parameters 7.2 Other input parameters

8 8 9

8 PREDICTION OF SOME OF THE INPUT PARAMETERS 8.1 Fugacity of CO2 8.2 pH 8.3 Humidity 8.4 Wall shear stress

11 11 12 14 15

9 INFORMATIVE REFERENCES

18

NORSOK standard

Page 1 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

FOREWORD NORSOK (The competitive standing of the Norwegian offshore sector) is the industry initiative to add value, reduce cost and lead time and eliminate unnecessary activities in offshore field developments and operations. The NORSOK standards are developed by the Norwegian petroleum industry as a part of the NORSOK initiative and supported by OLF (The Norwegian Oil Industry Association) and TBL (Federation of Norwegian Engineering Industries). NORSOK standards are administered and issued by NTS (Norwegian Technology Standards Institution). The purpose of NORSOK standards is to contribute to meet the NORSOK goals, e.g. by replacing individual oil company specifications and other industry guidelines and documents for use in existing and future petroleum industry developments. The NORSOK standards make extensive references to international standards. Where relevant, the contents of a NORSOK standard will be used to provide input to the international standardisation process. Subject to implementation into international standards, the NORSOK standard will be withdrawn. The computer program is informative.

INTRODUCTION This standard contains two parts as described below: 1. The Clauses 4, 5, 6, 7 and 8 in this standard acts as the user manual for the computer program. A description of the calculation model, the algorithms and the conditions for the corrosion rate calculations are given. In additions, methods and algorithms for calculation of essential input parameters to the corrosion rate calculations are given. 2. The computer program for corrosion rate calculations is available for downloading free of charge from the NTS/NORSOK Internet website (http://www.nts.no/norsok) or it may be procured from NTS, Oslo.

NORSOK standard

Page 2 of 18

CO2 corrosion rate calculation model ________________________________________________________

1

M-506 Rev. 1, June 1998

SCOPE

The scope of this standard is to present a method for calculation of corrosion rates in hydrocarbon production and process systems where the corrosive agent is CO2. The standard has primarily been developed for calculation of corrosion rates in topside piping systems and vessels, but the program may also be used for calculation of corrosion rates in pipeline systems and subsea production facilities.

2

NORMATIVE REFERENCES

The following standard includes provisions which, through reference in this text, constitute provisions of this NORSOK standard. Latest issue of the reference shall be used unless otherwise agreed. Other recognised standards may be used provided it can be shown that they meet or exceed the requirements of the standard referenced below. NORSOK standard M-001 “Material Selection”.

3

DEFINITIONS AND ABBREVIATIONS

3.1 Can

Definitions

Informative references May Shall

Should

Verbal form used for statements of possibility and capability, whether material, physical or casual. Shall mean informative in the application of NORSOK standards. Verbal form used to indicate a course of action permissible within the limits of the standard. Verbal form used to indicate requirements strictly to be followed in order to conform to the standard and from which no deviation is permitted, unless accepted by all involved parties. Verbal form used to indicate that among several possibilities one is recommended as particularly suitable, without mentioning or excluding others, or that a certain course of action is preferred but not necessarily required.

3.2

Symbols

A a CRt C(index) D FH2O Ftot f

- cross sectional area (m2) - fugacity coefficient - corrosion rate at temperature t (mm/y) - concentration of component - pipe diameter - water mass flow in humidity calculations - total mass flow in humidity calculations - friction factor

NORSOK standard

Page 3 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

f(pH)t fCO2 φ φc I k K(index) K(index) Kt λ µo µG µL µm µrelmax µw P pCO2 pH2O QG QL Re ρG ρL ρm ρo ρw S t Tc Tf T Tstd um uGS uLS

- the pH factor at temperature t - fugacity of CO2 (bar) - watercut - watercut at inversion point - ionic strength given in molar. - pipe roughness (m) - equilibrium constant used in pH calculations - constant used in viscosity calculations - constant for the temperature t used in corrosion rate calculations - liquid fraction - viscosity of oil (Ns/m2) - viscosity of gas (Ns/m2) - viscosity of liquid (Ns/m2) - mixed viscosity (Ns/m2) - maximum relative viscosity (relative to the oil) - viscosity of water (Ns/m2) - total system pressure (bar) - CO2 partial pressure (bar) - H2O vapour pressure - volumetric flow of gas (MSm3/d) - volumetric flow of liquid, i.e. liquid hydrocarbons and water, (Sm3/d) - Reynolds number - gas density (kg/m3) - liquid density (kg/m3) - mixed density (kg/m3) - oil density (kg/m3) - water density (kg/m3) - wall shear stress (Pa) - 20, 40, 60, 80, 90, 120 or 150°C - temperature given in °C - temperature given in °F - temperature given in Kelvin. - temperature given in Kelvin at standard conditions (60 °F/15,55 oC) - mixed velocity (m/s) - superficial velocities of gas (m/s) - superficial velocities of liquid (m/s)

4

PRINCIPLES FOR USE OF THE COMPUTER PROGRAM

The corrosion rate equations included in this standard describe the calculation model which shall apply, while the computer program itself is an optional aid which the users of the model may apply such that they possess an efficient tool to conduct corrosion rate calculations and parameter studies. This computer program is developed based on the corrosion rate model given as equations in this standard.

NORSOK standard

Page 4 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

The computer program is an aid in CO2 corrosion rate assessments, but the user of the computer program is responsible for the results and the final material selections and piping and equipment design. Therefore the user of the program must perform a critical evaluation of all results and the applicability of these in each case. Corrosion rate calculation, is only one element in a material selection process. Other essential factors are uncertainty in input data for corrosion rate calculations, construction and commissioning conditions, consideration of normal and upset operating conditions, actual corrosivity of produced fluids, scale, wax, inhibitor efficiency and geometry of corrosion attacks. These and other factors may influence the actual corrosion rates considerably, and be more important than any uncertainty in the corrosion rate calculations. As the computer program is distributed electronically and may be used on computers and program versions outside the control of NTS/NORSOK, users of the computer program are sole responsible to verify that the computer calculations are in accordance with the equations in this standard. This standard provides an introduction to the corrosion rate computer program. It also gives limitations and requirements to input parameters and results. Instructions for running the program are given in the help functions to the program. The program covers only calculation of corrosion rates where CO2 is the corrosive agent. It does not include additional effects of other constituents which may influence the corrosivity, e.g. contamination’s of O2, H2S etc. If such constituents are present, which is common in e.g. produced water systems, these effects must be evaluated separately. Principles for materials selection is given in NORSOK standard M-001 “Material Selection”. The requirements in NORSOK M-001 shall be used when generating input data and when interpreting results from this CO2 corrosion rate calculation standard. It is important to note that this standard and computer program may use or generate data which are outside the limits of NORSOK M-001. One example is corrosion inhibitor efficiency, where NORSOK M-001 provides maximum allowable values, while the computer program accepts all values from 0 to 100%. In case of conflict, NORSOK M-001 shall apply when selecting materials.

5

DESCRIPTION OF THE CO2 CORROSION RATE MODEL

5.1 General The model is an empirical corrosion rate model for carbon steel in water containing CO2 at different temperatures, pH's, CO2 fugacities and wall shear stresses. It is based on flow-loop experiments at temperatures from 20-160°C. A large amount of data at various temperatures, CO2 fugacities, pH's and wall shear stresses are used. The main bulk of the flow loop tests used in developing the calculation model is taken from the Kjeller Sweet Corrosion research program at Institute for Energy Technology in Norway. The main principles for the testing is described in a paper by Dugstad et. al. /1/. Most of the data directly used in the modelling work has been generated after this paper /1/ was presented.

NORSOK standard

Page 5 of 18

CO2 corrosion rate calculation model ________________________________________________________ 5.2

M-506 Rev. 1, June 1998

The corrosion model

5.2.1 General The following general equation of the CO2 corrosion rate for carbon steel at each of the temperatures (t); 20, 40, 60, 80, 90, 120 and 150°C is used: CRt = Kt x fCO20,62 x (S/19) 0,146 + 0,0324 log (fCO2) x f(pH)t where:

Kt fCO2 S f(pH)t

(mm/year)

- Constant for the temperature t - the fugacity of CO2 (bar) - Wall shear stress (Pa) - The pH factor at temperature t

The corrosion rate between temperatures where a constant Kt has been generated, is found by a linear extrapolation between the calculated corrosion rate at the temperature above and below the desired temperature. The constant Kt is given in the table below. Table 5.1 - Constant Kt Temperature °C

Kt

20 40 60 80 90 120 150

4,762 8,927 10,695 9,949 6,250 7,770 5,203

The effect of pH is given in the table below.

NORSOK standard

Page 6 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 5.2 - pH function Temperatur e

pH

20 oC 20 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 2,0676 - (0,2309 x pH) f(pH) = 5,1885 - (1,2353 x pH) + (0,0708 x pH2)

40 oC 40 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 2,0676 - (0,2309 x pH) f(pH) = 5,1885 - (1,2353 x pH) + (0,0708 x pH2)

60 oC 60 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 1,836 - (0,1818 x pH) f(pH) = 15,444 - (6,1291 x pH) + (0,8204 x pH2) - (0,0371 x pH3)

80 oC 80 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 2,6727 - (0,3636 x pH) f(pH) = 331,68 x e(-1,2618 x pH)

90 oC 90 oC 90 oC

3,5< pH < 4,57 4,57< pH < 5,62 5,62 < pH < 6,5

f(pH) = 3,1355 - (0,4673 x pH) f(pH) = 21254 x e(-2,1811 x pH) f(pH) = 0,4014 - (0,0538 x pH)

120 oC 120 oC 120 oC

3,5 < pH < 4,3 4,3 < pH < 5 5 < pH < 6,5

f(pH) = 1,5375 - (0,125 x pH) f(pH) = 5,9757 - (1,157 x pH) f(pH) = 0,546125 - (0,071225 x pH)

150 oC 150 oC 150 oC

3,5 < pH < 3,8 3,8 < pH < 5 5 < pH < 6,5

f(pH) = 1 f(pH) = 17,634 - (7,0945 x pH) + (0,715 x pH2) f(pH) = 0,037

5.3

f(pH)

The effect of glycol and corrosion inhibitors

The effect of glycol on the corrosion rate is calculated as a reduction factor /2/: • Glycol reduction factor = 10 1,6 (log (100-wt%Glycol)-2)

for less than 95 weight-% glycol.

• For > 95 weight-% glycol, the glycol reduction factor is set to 0,008. The effect of corrosion inhibitors is entered directly as a reduction factor in the computer program. When both addition of corrosion inhibitors and glycol is entered into the computer program, the one effect giving the greatest corrosion rate reduction factor will be used for calculation of the resulting corrosion rate, i.e. the two effects will not be combined.

NORSOK standard

Page 7 of 18

CO2 corrosion rate calculation model ________________________________________________________

6

M-506 Rev. 1, June 1998

STRUCTURE OF THE COMPUTER PROGRAMME

The computer program has a main dialogue box, denoted as the “Main Menu”, where all corrosion rate calculations can be performed. All input parameters can be entered into the program directly at this stage for point calculations. As options and support functions, it is possible to calculate several of the important parameters by selecting optional dialogue boxes. Such options are: • pH calculations • shear stress calculations • humidity calculations for gas systems (not an input parameter used in the calculations, but essential in evaluating risk for corrosion in gas systems) These program options are included in order to generate adequate input data for corrosion rate prediction based on data normally presented in process flow diagrams and design basis documents. The support program options are prepared to give adequate accuracy for corrosion rate calculations, and shall not be used for other purposes, e.g. genuine process, scale or flow calculations. In the clauses below, the input parameters and the corrosion rate calculation model are explained. Additionally, the support functions for calculation of some of the input parameters are explained. Other support functions, such as “Parameter study”, “Accumulated corrosion”, saving of data, print of data etc. are not specifically explained in this standard, but are covered by the “Help” function provided in the computer program.

7

INPUT PARAMETERS

7.1

Basic input parameters

The basic input parameters for the CO2 corrosion model for carbon steel are given in table 7.1. The allowed units and ranges are also given.

NORSOK standard

Page 8 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 7.1 - Basic input parameters Parameter Temperature

Units °C °F bar psi kmole/h bar psi mole% kmole/h Pa

Total pressure Total mass flow CO2 fugacity in the gas phase Wall shear stress

Range 20-150 68-302 1-1000 14,5-14500 10-3 - 106 0-10 0-145 variable variable 1-150

pH

3,5-6,5

Glycol concentration Inhibitor efficiency

weight-% %

0-100 0-100

Comments

Only relevant when CO2 is given in kmole/h. The CO2 partial pressure must be < the total pressure. The allowed ranges of mole% and kmole/h CO2 are dependent on the total pressure Can be calculated by use of other input parameters - see 7.2.1 Can be calculated by use of other input parameters - see 7.2.2 Ref. NORSOK M-001

7.2

Other input parameters

7.2.1

Input parameters for wall shear stress calculations

To calculate the wall shear stress, the input parameters given in table 7.2, are as a minimum required. Table 7.2. Input parameters for simplified calculation of wall shear stress Parameter Temperature Total pressure Superficial liquid velocity/ Liquid flow Superficial gas velocity/ Gas flow Watercut, Φ Diameter (ID)

Units °C °F bar psi m/s Sm³/d m/s MSm³/d % mm

Range 5 - 150 41 - 302 1 - 1000 14,5 - 14500 0 - 20 (depends on ID) 0 - 40 (depends on ID) 0 - 100 0-∞

Comments

Requirement: turbulent flow, i.e. Re > 2300 Requirement: turbulent flow, i.e. Re > 2300

Requirement: turbulent flow, i.e. Re > 2300

For more accurate wall shear stress calculations, the input parameters given in table 7.3 should also be used.

NORSOK standard

Page 9 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 7.3 - Input parameters for accurate calculation of wall shear stress. Parameter Roughness Compressibility Specific gravity of gas relative to air Water density, ρw Oil density, ρo Gas density, ρw Water viscosity, µw Oil viscosity, µo Gas viscosity, µG

Units µm

kg/m³ kg/m³ kg/m³ cp N s/m² cp N s/m² cp N s/m²

Water cut at inversion point, φc Max. relative liquid viscosity, µrelmax

7.2.2

Range 0 - 100 0,8 - 1 0,5 - 1 995 - 1050 600 - 1100 1 - 1700 0,17 - 1,1 0,00017 - 0,0011 0,2 - 200 0,0002 - 0,2 0,02 - 0,06 0,00002 - 0,00006 0,3 - 0,9 1 - 100

Default value 50 0,9 0,8 1024 850 calculated calculated 1,1 0,03 0,5 7,06

Input parameters for pH calculations

To predict the pH in the condensed water or formation water, the parameters given in table 7.4 are needed. Table 7.4 - Input parameters for pH calculations Parameter

Unit

Range

Temperature

°C °F bar psi kmole/h

5-150 41-302 1-1000 14,5-14500 10-3 - 106

Total pressure Total mass flow CO2 fugacity

bar psi mole% kmole/h Bicarbonate (HCO3-) mg/l mM Ionic strength/ salinity g/l M

7.2.3

0-10 0-145 variable variable 0-20000 0-327 0-175 0-3

Default Comments values

0

Only relevant when CO2 is given in kmole/h. The CO2 partial pressure must be < the total pressure. The allowed ranges of mole% and kmole/h CO2 are dependent on the total pressure. Default values for formation water

50

Default values for formation water

Humidity calculations

NORSOK standard

Page 10 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 7.5. Input parameters for humidity calculation Parameter Temperature Total pressure Water mass flow Total mass flow

8

Unit °C °F bar psi kmole/h kmole/h

Range -16 - 200 3,2 - 392 1-1000 14,5-14500 10-3 - 106 10-3 - 106

Comments

The water mass flow must be < the total mass flow

PREDICTION OF SOME OF THE INPUT PARAMETERS

8.1 Fugacity of CO2 At high pressures gases are not ideal. To compensate for this, the partial pressure of a gas is multiplied by a fugacity constant. The real CO2 pressure can then be expressed as: fCO2 = a

.

pCO2

where: fCO2 = the fugacity of CO2 (bar) a = fugacity constant which depends on pressure and temperature pCO2 = CO2 partial pressure (bar) The CO2 partial pressure is found by one of the following expressions: pCO2 = (mole% CO2 in the gas phase/ 100% ) . P or

pCO2 = mass flow of CO2 in the gas phase (kmole/h) . P total mass flow in the gas phase (kmole/h)

where P is the total pressure in the system. The fugacity coefficient is given as /2/: a = 10

P( 0,0031 - 1,4/T)

for P < 250 bar

a = 10

250(0,0031 - 1,4/T)

for P > 250 bar

where T is the temperature in °K and P is the total pressure given in bar. The total pressure is set to 250 bar in the fugacity constant for all pressures above 250.

NORSOK standard

Page 11 of 18

CO2 corrosion rate calculation model ________________________________________________________ 8.2

pH

8.2.1

General considerations

M-506 Rev. 1, June 1998

The program contains a pH calculation module. The pH in both condensed water and formation water can be calculated. Some essential general considerations relevant for pH assessment is given below. The reported pH in water analyses is usually measured after depressurisation and atmospheric exposure of the sample. Such pH’s give no information about the in situ pH which is a requisite for the corrosion rate evaluation. The in situ pH has to be determined by calculations which take into account the three controlling buffer systems CO2 /HCO3 , H2S/HS- and CH3COOH/CH3COO-. The buffer system CH3COOH/CH3COO- can be extended to include all the other organic acids that may influence the pH determination as these acids have similar dissociation constants. The bicarbonate concentration, which is used for pH calculation, is routinely determined by titration and the reported value is set equal to the alkalinity. This is correct as long as the H2S concentration is low and the system does not contain acetic acid. For waters containing significant amount of organic acids, the reported bicarbonate concentration requires correction because organic acids contributes to the measured value of total alkalinity. The correction will be 2/3 of the organic acid concentration assuming that the end point pH of the titration is 4.3. Lower pH requires a higher fraction. More details about the interpretation of the water analysis and the determination of pH can be found in the EFC publication number 16 /3/. 8.2.2 Calculation of pH The routine for calculation of pH is based on the following chemical reactions and equilibrium constants: C CO2 (g) = CO2 (aq)

K

H

=

CO 2

p

CO 2

C CO2 (aq) + H2O = H2CO3

K = 0

H CO 2 3

C

CO 2

C

−

C

HCO

H2CO3 = H+ + HCO3-

3

K = 1

C

H CO 2 3

C

2−

C

CO

HCO3- = H+ + CO32-

+ H

3

K = 2

+ H

C

− HCO 3

NORSOK standard

Page 12 of 18

CO2 corrosion rate calculation model ________________________________________________________ H2O = H+ + OH-

=C

K

+

W H

C

M-506 Rev. 1, June 1998

− OH

The system has to be electro-neutral, which can be described by the following equation: C

+

+C + = C

Na

H

−

+ 2C

HCO

2−

+C

CO 3

−

+C −

OH

Cl

3

It is assumed that bicarbonate is added as sodium bicarbonate (NaHCO3). It is also assumed that no other salts than sodium bicarbonate and sodium chloride (NaCl) are present in the solution. These salts will dissolve as follows: NaCl = Na+ + ClNaHCO3 = Na+ + HCO3Based on these assumptions, the amount of sodium bicarbonate equals the difference in the concentrations of sodium and chloride as shown below. The mass balance for bicarbonate will therefore be as follows: C

0. Bicarb

=C

+

−C

−

Cl

Na

C0,Bicarb equals the initial amount of sodium bicarbonate. By combining the equations for the equilibrium constants with the required electro-neutrality and the mass balance for bicarbonate one get the following expression for the concentration of the Hydrogen cation: 3

C

+ H

+C

2 0 , Bicarb

C

+ H

− (K K K p H

0

+ K )C

1 CO

W

2

+ H

− 2K K K K p H

0

1

2

=0

CO 2

This equation is solved by using the Newton's Method. The pH in a condensed water system saturated with iron carbonate can also be calculated. Based on a similar deduction as above, the equation becomes:

4 2K 3 2 SP C + C + C C + + + − ( KH K0 K1 pCO + KW )C + − 2KH K0 K1 K2 pCO = 0 0, Bicarb K K K K p H H H H H 0 1 2 CO2 2 2 where KSP is the equilibrium constant of iron carbonate. 8.2.3 Equilibrium constants The equilibrium constant and the forward reaction rate constant for the carbon dioxide hydration were given by Palmer and van Eldik /4/: K0 = 0,00258

NORSOK standard

Page 13 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

The equilibrium constant for iron carbonate was taken from IUPAC /5/: KSP = 10

-(10,13 + 0,0182Tc)

molar2 where Tc is the temperature in oC.

The rest of the equilibrium constants were given by Oddo and Tomson /6/:

K

H

=

14,5 × 10 1,00258

− ( 2 ,27 + 5, 65 × 10

− ( 6,41 − 1,594 × 10

K = 387,6 × 10 1

− (10, 61− 4 ,97 × 10

K = 10 2

−3

−3

−3

T − 8,06 × 10 f

T + 8,52 × 10 f

T + 1,331 × 10 f

−6 2 T + 0,075 I ) f

molar / bar

−6 2 −5 1/ 2 + 0,1180 I ) T − 3,07 × 10 P − 0,4772 I f

−5 2 −5 1/ 2 + 0,3466 I ) T − 2 , 624 × 10 P − 1,166 I f

molar

molar

Tf : temperature given in °F. P : the pressure given in psi. I : the ionic strength given in molar. The equation for the equilibrium constant for the dissociation of water was based on data given by Delahay/7/: − ( 29 ,3868 − 0,0737549 T + 7 ,47881x10

K

w

= 10

−5 2 T )

molar

2

T: Temperature in Kelvin. 8.3 Humidity A prerequisite for corrosion to occur is that there is liquid water present in the system. In gas systems, an essential assessment is to determine if the presence of condensed water is possible. The program therefore includes a support function to calculate humidity in pure water /8/, i.e. in systems without glycol. Humidity (%) = 100 (P . FH2O)/(pH2O . Ftot) Where P = Total pressure pH2O = Water vapour pressure FH2O = Water mass flow Ftot = Total mass flow The dew point temperature (Tdew) equals the temperature where the humidity is 100%.

NORSOK standard

Page 14 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

8.4 Wall shear stress Wall shear stress is one of the parameters needed for calculation of corrosion rate. In the model, the mean wall shear stress in straight pipe sections is used. Obstacles and other geometrical changes in the flow will give rise to higher shear stresses than calculated by this program. Further, different flow regimes and geometrical obstacles may generate shear stress fluctuations where the shear stress peaks may be considerably higher than the average shear stress. High shear stress may cause mesa attacks, with corrosion rates significantly higher than what is estimated by this computer program. It is not the objective of this computer program to cover all such eventualities, and the user of the program must evaluate the flow effect in each system/part of a system based on expertise and available experience and documentation. The mean wall shear on the wall at medium to high superficial velocities of one or both of the liquid and gas velocities: S = 0,5 x ρm x f x um2

(Pa)

where the friction factor, f, can be expressed as:

f

k = 0,001375 1 + 20000 D

+ 10

6

µ

m ρ u D m m

0,33

k = Pipe roughness and D = Pipe diameter Mixture density, velocity and viscosity is expressed as: ρm = ρL λ + ρG (1 - λ) ρL = φ ρw + ρo (1 - λ) ρG = 2,7 . 14,5 . 16,018 . P . specific gravity/(Z . (460 + Tf)) φ = water cut and Z = compressibility of the gas um = uLs + uGs The liquid is considered incompressible: uLs = QL / A The gas superficial velocity is: uGs = (QG / A) Z (T/Tstd) µm = µL x λ + µG (1 - λ)

λ =

QL

QL + QG

This model /9/ is verified for medium/high flow rates by tests. If water is present the viscosity of the liquid is found as follows:

NORSOK standard

Page 15 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

The effective viscosity of a kinetically stable oil/water mixture depends on the watercut /10/. Preferably the maximum magnitude of viscosity and the corresponding watercut should be known. The viscosity of the oil wet region, i.e. below the inversion point in a dispersed flow, can be represented as:

µ

L

=

µ

0

1

φ K

+

φ K 0

0

−

1 ,1 8 7

2 ,5

(Ns/m2 )

µo : viscosity of oil (Ns/m2 ) The value of K0 for the maximum relative viscosity µrelmax (relative to the oil) and corresponding watercut at the inversion point, φc, is equal to : K

0

φ

=

1

1 ,1 8 7

−

c

1 µ rel m ax

0 ,4

If not known, data for a medium viscosity oil/water dispersion will be used. This dispersion exhibits a maximum value of relative viscosity = 7,06 at a watercut of 0,5. The oil viscosity is equal to 0,0011 Ns/m2 at 60°C and the water viscosity is equal to 0,00046 Ns/m2. Above the inversion point, the viscosity of any dispersion is given as:

µ

L

=

µ

w

1− φ K + w 1 1− φ 1,1 8 7 − K w

2 ,5

(Ns/m2 )

µw : viscosity of water (Ns/m2 ) Where: K

w

= 1 ,1 8 7

NORSOK standard

1

φ

1

−

−

R µ rel m ax

c

0 ,4

Page 16 of 18

CO2 corrosion rate calculation model ________________________________________________________

R =

µ

M-506 Rev. 1, June 1998

water µ oil

The viscosity of water is as default given as function of temperature, Tc, given in oC /8/: 0 - 20 oC:

µ

2 1301/ ( 998,333 + 8,1855( T − 20 ) + 0,00585( T − 20 ) ) − 1,30233 c c

w

= 10

⋅ 10

−3

(Ns/m2 )

20 - 150 oC (the formula is strictly only valid up to 100 oC, but used up to 150 oC in this context): 2 (1,3272(20−T ) −0,001053(T −20) )/(T +105) c c

µ = 1002 , (10 w

−3 ) 10

(Ns/m2 )

For the medium viscosity oil at 60oC , R is equal to 0,42.

NORSOK standard

Page 17 of 18

CO2 corrosion rate calculation model ________________________________________________________

9

M-506 Rev. 1, June 1998

INFORMATIVE REFERENCES

/1/

A. Dugstad, L. Lunde, K.Videm “Parametric study of CO2 corrosion of carbon steel” NACECorrosion-94 paper No 14. /2/ C. de Waard, U. Lotz, D.E.Milliams "Predictive model for CO2 Corrosion engineering in wet natural gas pipelines", Corrosion December 1991 pp. 976 /3/ Guidelines on materials requirement for carbon and low alloy steels for H2S-containing environments in oil and gas production, European Federation of corrosion publication number 16, the Institute of Materials, 1995 /4/ D. A. Palmer and R. V. Eldik, Chem. Rev., Vol. 83, p. 651, 1983. /5/ IUPAC: Chemical Data Series No 21. Stability constants of Metal-Ion Complexes. Par A: Inorganic ligands. Pergamon Press. /6/ J. E. Oddo and M. B. Tomson, "Simplified Calculation of CaCO3 Saturation at High Temperatures and Pressures in Brine Solutions". SPE of AIME, pp. 1583, 1982. /7/ P. Delahay, “Implication of the Kinetics of Ionic Dissociation with regard to some Electrochemical Process-application to Polarography.” I.Am.Chem.Sic, 74, 1952 pp 3497. /8/ D. R. Lide, “CRC Handbook of Chemistry and Physics” 66th edition, CRC Press Inc. 19851986 /9/ A. E. Dukler, M. Wicks III, R.G. Cleveland, Frictional pressure drop in two phase flow. An approach through similarity analysis, A.I.Ch.E. Journal, Vol. 10, No 1, January 1964 /10/ H. Kvandal, T. Søntvedt, Frictional pressure loss for stable oil-water emulsions in pipeflow. Symposium on two phase flow modelling and experimentation, Rome 1995.

NORSOK standard

Page 18 of 18

View more...
CO2 CORROSION RATE CALCULATION MODEL

M-506 Rev. 1, June 1998

This NORSOK standard is developed by NTS with broad industry participation. Please note that whilst every effort has been made to ensure the accuracy of this standard, neither OLF nor TBL or any of their members will assume liability for any use thereof. NTS is responsible for the administration and publication of this standard. Norwegian Technology Standards Institution Oscarsgt. 20, Postbox 7072 Majorstua N-0306 Oslo, NORWAY Telephone: + 47 22 59 67 00 Fax: + 47 22 59 67 29 Email: [email protected] Website: http://www.nts.no/norsok Copyrights reserved

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

CONTENTS FOREWORD INTRODUCTION

2 2

1 SCOPE

3

2 NORMATIVE REFERENCES

3

3 DEFINITIONS AND ABBREVIATIONS 3.1 Definitions 3.2 Symbols

3 3 3

4 PRINCIPLES FOR USE OF THE COMPUTER PROGRAM

4

5 DESCRIPTION OF THE CO2 CORROSION RATE MODEL 5.1 General 5.2 The corrosion model 5.3 The effect of glycol and corrosion inhibitors

5 5 6 7

6 STRUCTURE OF THE COMPUTER PROGRAMME

8

7 INPUT PARAMETERS 7.1 Basic input parameters 7.2 Other input parameters

8 8 9

8 PREDICTION OF SOME OF THE INPUT PARAMETERS 8.1 Fugacity of CO2 8.2 pH 8.3 Humidity 8.4 Wall shear stress

11 11 12 14 15

9 INFORMATIVE REFERENCES

18

NORSOK standard

Page 1 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

FOREWORD NORSOK (The competitive standing of the Norwegian offshore sector) is the industry initiative to add value, reduce cost and lead time and eliminate unnecessary activities in offshore field developments and operations. The NORSOK standards are developed by the Norwegian petroleum industry as a part of the NORSOK initiative and supported by OLF (The Norwegian Oil Industry Association) and TBL (Federation of Norwegian Engineering Industries). NORSOK standards are administered and issued by NTS (Norwegian Technology Standards Institution). The purpose of NORSOK standards is to contribute to meet the NORSOK goals, e.g. by replacing individual oil company specifications and other industry guidelines and documents for use in existing and future petroleum industry developments. The NORSOK standards make extensive references to international standards. Where relevant, the contents of a NORSOK standard will be used to provide input to the international standardisation process. Subject to implementation into international standards, the NORSOK standard will be withdrawn. The computer program is informative.

INTRODUCTION This standard contains two parts as described below: 1. The Clauses 4, 5, 6, 7 and 8 in this standard acts as the user manual for the computer program. A description of the calculation model, the algorithms and the conditions for the corrosion rate calculations are given. In additions, methods and algorithms for calculation of essential input parameters to the corrosion rate calculations are given. 2. The computer program for corrosion rate calculations is available for downloading free of charge from the NTS/NORSOK Internet website (http://www.nts.no/norsok) or it may be procured from NTS, Oslo.

NORSOK standard

Page 2 of 18

CO2 corrosion rate calculation model ________________________________________________________

1

M-506 Rev. 1, June 1998

SCOPE

The scope of this standard is to present a method for calculation of corrosion rates in hydrocarbon production and process systems where the corrosive agent is CO2. The standard has primarily been developed for calculation of corrosion rates in topside piping systems and vessels, but the program may also be used for calculation of corrosion rates in pipeline systems and subsea production facilities.

2

NORMATIVE REFERENCES

The following standard includes provisions which, through reference in this text, constitute provisions of this NORSOK standard. Latest issue of the reference shall be used unless otherwise agreed. Other recognised standards may be used provided it can be shown that they meet or exceed the requirements of the standard referenced below. NORSOK standard M-001 “Material Selection”.

3

DEFINITIONS AND ABBREVIATIONS

3.1 Can

Definitions

Informative references May Shall

Should

Verbal form used for statements of possibility and capability, whether material, physical or casual. Shall mean informative in the application of NORSOK standards. Verbal form used to indicate a course of action permissible within the limits of the standard. Verbal form used to indicate requirements strictly to be followed in order to conform to the standard and from which no deviation is permitted, unless accepted by all involved parties. Verbal form used to indicate that among several possibilities one is recommended as particularly suitable, without mentioning or excluding others, or that a certain course of action is preferred but not necessarily required.

3.2

Symbols

A a CRt C(index) D FH2O Ftot f

- cross sectional area (m2) - fugacity coefficient - corrosion rate at temperature t (mm/y) - concentration of component - pipe diameter - water mass flow in humidity calculations - total mass flow in humidity calculations - friction factor

NORSOK standard

Page 3 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

f(pH)t fCO2 φ φc I k K(index) K(index) Kt λ µo µG µL µm µrelmax µw P pCO2 pH2O QG QL Re ρG ρL ρm ρo ρw S t Tc Tf T Tstd um uGS uLS

- the pH factor at temperature t - fugacity of CO2 (bar) - watercut - watercut at inversion point - ionic strength given in molar. - pipe roughness (m) - equilibrium constant used in pH calculations - constant used in viscosity calculations - constant for the temperature t used in corrosion rate calculations - liquid fraction - viscosity of oil (Ns/m2) - viscosity of gas (Ns/m2) - viscosity of liquid (Ns/m2) - mixed viscosity (Ns/m2) - maximum relative viscosity (relative to the oil) - viscosity of water (Ns/m2) - total system pressure (bar) - CO2 partial pressure (bar) - H2O vapour pressure - volumetric flow of gas (MSm3/d) - volumetric flow of liquid, i.e. liquid hydrocarbons and water, (Sm3/d) - Reynolds number - gas density (kg/m3) - liquid density (kg/m3) - mixed density (kg/m3) - oil density (kg/m3) - water density (kg/m3) - wall shear stress (Pa) - 20, 40, 60, 80, 90, 120 or 150°C - temperature given in °C - temperature given in °F - temperature given in Kelvin. - temperature given in Kelvin at standard conditions (60 °F/15,55 oC) - mixed velocity (m/s) - superficial velocities of gas (m/s) - superficial velocities of liquid (m/s)

4

PRINCIPLES FOR USE OF THE COMPUTER PROGRAM

The corrosion rate equations included in this standard describe the calculation model which shall apply, while the computer program itself is an optional aid which the users of the model may apply such that they possess an efficient tool to conduct corrosion rate calculations and parameter studies. This computer program is developed based on the corrosion rate model given as equations in this standard.

NORSOK standard

Page 4 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

The computer program is an aid in CO2 corrosion rate assessments, but the user of the computer program is responsible for the results and the final material selections and piping and equipment design. Therefore the user of the program must perform a critical evaluation of all results and the applicability of these in each case. Corrosion rate calculation, is only one element in a material selection process. Other essential factors are uncertainty in input data for corrosion rate calculations, construction and commissioning conditions, consideration of normal and upset operating conditions, actual corrosivity of produced fluids, scale, wax, inhibitor efficiency and geometry of corrosion attacks. These and other factors may influence the actual corrosion rates considerably, and be more important than any uncertainty in the corrosion rate calculations. As the computer program is distributed electronically and may be used on computers and program versions outside the control of NTS/NORSOK, users of the computer program are sole responsible to verify that the computer calculations are in accordance with the equations in this standard. This standard provides an introduction to the corrosion rate computer program. It also gives limitations and requirements to input parameters and results. Instructions for running the program are given in the help functions to the program. The program covers only calculation of corrosion rates where CO2 is the corrosive agent. It does not include additional effects of other constituents which may influence the corrosivity, e.g. contamination’s of O2, H2S etc. If such constituents are present, which is common in e.g. produced water systems, these effects must be evaluated separately. Principles for materials selection is given in NORSOK standard M-001 “Material Selection”. The requirements in NORSOK M-001 shall be used when generating input data and when interpreting results from this CO2 corrosion rate calculation standard. It is important to note that this standard and computer program may use or generate data which are outside the limits of NORSOK M-001. One example is corrosion inhibitor efficiency, where NORSOK M-001 provides maximum allowable values, while the computer program accepts all values from 0 to 100%. In case of conflict, NORSOK M-001 shall apply when selecting materials.

5

DESCRIPTION OF THE CO2 CORROSION RATE MODEL

5.1 General The model is an empirical corrosion rate model for carbon steel in water containing CO2 at different temperatures, pH's, CO2 fugacities and wall shear stresses. It is based on flow-loop experiments at temperatures from 20-160°C. A large amount of data at various temperatures, CO2 fugacities, pH's and wall shear stresses are used. The main bulk of the flow loop tests used in developing the calculation model is taken from the Kjeller Sweet Corrosion research program at Institute for Energy Technology in Norway. The main principles for the testing is described in a paper by Dugstad et. al. /1/. Most of the data directly used in the modelling work has been generated after this paper /1/ was presented.

NORSOK standard

Page 5 of 18

CO2 corrosion rate calculation model ________________________________________________________ 5.2

M-506 Rev. 1, June 1998

The corrosion model

5.2.1 General The following general equation of the CO2 corrosion rate for carbon steel at each of the temperatures (t); 20, 40, 60, 80, 90, 120 and 150°C is used: CRt = Kt x fCO20,62 x (S/19) 0,146 + 0,0324 log (fCO2) x f(pH)t where:

Kt fCO2 S f(pH)t

(mm/year)

- Constant for the temperature t - the fugacity of CO2 (bar) - Wall shear stress (Pa) - The pH factor at temperature t

The corrosion rate between temperatures where a constant Kt has been generated, is found by a linear extrapolation between the calculated corrosion rate at the temperature above and below the desired temperature. The constant Kt is given in the table below. Table 5.1 - Constant Kt Temperature °C

Kt

20 40 60 80 90 120 150

4,762 8,927 10,695 9,949 6,250 7,770 5,203

The effect of pH is given in the table below.

NORSOK standard

Page 6 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 5.2 - pH function Temperatur e

pH

20 oC 20 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 2,0676 - (0,2309 x pH) f(pH) = 5,1885 - (1,2353 x pH) + (0,0708 x pH2)

40 oC 40 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 2,0676 - (0,2309 x pH) f(pH) = 5,1885 - (1,2353 x pH) + (0,0708 x pH2)

60 oC 60 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 1,836 - (0,1818 x pH) f(pH) = 15,444 - (6,1291 x pH) + (0,8204 x pH2) - (0,0371 x pH3)

80 oC 80 oC

3,5 < pH < 4,6 4,6 < pH < 6,5

f(pH) = 2,6727 - (0,3636 x pH) f(pH) = 331,68 x e(-1,2618 x pH)

90 oC 90 oC 90 oC

3,5< pH < 4,57 4,57< pH < 5,62 5,62 < pH < 6,5

f(pH) = 3,1355 - (0,4673 x pH) f(pH) = 21254 x e(-2,1811 x pH) f(pH) = 0,4014 - (0,0538 x pH)

120 oC 120 oC 120 oC

3,5 < pH < 4,3 4,3 < pH < 5 5 < pH < 6,5

f(pH) = 1,5375 - (0,125 x pH) f(pH) = 5,9757 - (1,157 x pH) f(pH) = 0,546125 - (0,071225 x pH)

150 oC 150 oC 150 oC

3,5 < pH < 3,8 3,8 < pH < 5 5 < pH < 6,5

f(pH) = 1 f(pH) = 17,634 - (7,0945 x pH) + (0,715 x pH2) f(pH) = 0,037

5.3

f(pH)

The effect of glycol and corrosion inhibitors

The effect of glycol on the corrosion rate is calculated as a reduction factor /2/: • Glycol reduction factor = 10 1,6 (log (100-wt%Glycol)-2)

for less than 95 weight-% glycol.

• For > 95 weight-% glycol, the glycol reduction factor is set to 0,008. The effect of corrosion inhibitors is entered directly as a reduction factor in the computer program. When both addition of corrosion inhibitors and glycol is entered into the computer program, the one effect giving the greatest corrosion rate reduction factor will be used for calculation of the resulting corrosion rate, i.e. the two effects will not be combined.

NORSOK standard

Page 7 of 18

CO2 corrosion rate calculation model ________________________________________________________

6

M-506 Rev. 1, June 1998

STRUCTURE OF THE COMPUTER PROGRAMME

The computer program has a main dialogue box, denoted as the “Main Menu”, where all corrosion rate calculations can be performed. All input parameters can be entered into the program directly at this stage for point calculations. As options and support functions, it is possible to calculate several of the important parameters by selecting optional dialogue boxes. Such options are: • pH calculations • shear stress calculations • humidity calculations for gas systems (not an input parameter used in the calculations, but essential in evaluating risk for corrosion in gas systems) These program options are included in order to generate adequate input data for corrosion rate prediction based on data normally presented in process flow diagrams and design basis documents. The support program options are prepared to give adequate accuracy for corrosion rate calculations, and shall not be used for other purposes, e.g. genuine process, scale or flow calculations. In the clauses below, the input parameters and the corrosion rate calculation model are explained. Additionally, the support functions for calculation of some of the input parameters are explained. Other support functions, such as “Parameter study”, “Accumulated corrosion”, saving of data, print of data etc. are not specifically explained in this standard, but are covered by the “Help” function provided in the computer program.

7

INPUT PARAMETERS

7.1

Basic input parameters

The basic input parameters for the CO2 corrosion model for carbon steel are given in table 7.1. The allowed units and ranges are also given.

NORSOK standard

Page 8 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 7.1 - Basic input parameters Parameter Temperature

Units °C °F bar psi kmole/h bar psi mole% kmole/h Pa

Total pressure Total mass flow CO2 fugacity in the gas phase Wall shear stress

Range 20-150 68-302 1-1000 14,5-14500 10-3 - 106 0-10 0-145 variable variable 1-150

pH

3,5-6,5

Glycol concentration Inhibitor efficiency

weight-% %

0-100 0-100

Comments

Only relevant when CO2 is given in kmole/h. The CO2 partial pressure must be < the total pressure. The allowed ranges of mole% and kmole/h CO2 are dependent on the total pressure Can be calculated by use of other input parameters - see 7.2.1 Can be calculated by use of other input parameters - see 7.2.2 Ref. NORSOK M-001

7.2

Other input parameters

7.2.1

Input parameters for wall shear stress calculations

To calculate the wall shear stress, the input parameters given in table 7.2, are as a minimum required. Table 7.2. Input parameters for simplified calculation of wall shear stress Parameter Temperature Total pressure Superficial liquid velocity/ Liquid flow Superficial gas velocity/ Gas flow Watercut, Φ Diameter (ID)

Units °C °F bar psi m/s Sm³/d m/s MSm³/d % mm

Range 5 - 150 41 - 302 1 - 1000 14,5 - 14500 0 - 20 (depends on ID) 0 - 40 (depends on ID) 0 - 100 0-∞

Comments

Requirement: turbulent flow, i.e. Re > 2300 Requirement: turbulent flow, i.e. Re > 2300

Requirement: turbulent flow, i.e. Re > 2300

For more accurate wall shear stress calculations, the input parameters given in table 7.3 should also be used.

NORSOK standard

Page 9 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 7.3 - Input parameters for accurate calculation of wall shear stress. Parameter Roughness Compressibility Specific gravity of gas relative to air Water density, ρw Oil density, ρo Gas density, ρw Water viscosity, µw Oil viscosity, µo Gas viscosity, µG

Units µm

kg/m³ kg/m³ kg/m³ cp N s/m² cp N s/m² cp N s/m²

Water cut at inversion point, φc Max. relative liquid viscosity, µrelmax

7.2.2

Range 0 - 100 0,8 - 1 0,5 - 1 995 - 1050 600 - 1100 1 - 1700 0,17 - 1,1 0,00017 - 0,0011 0,2 - 200 0,0002 - 0,2 0,02 - 0,06 0,00002 - 0,00006 0,3 - 0,9 1 - 100

Default value 50 0,9 0,8 1024 850 calculated calculated 1,1 0,03 0,5 7,06

Input parameters for pH calculations

To predict the pH in the condensed water or formation water, the parameters given in table 7.4 are needed. Table 7.4 - Input parameters for pH calculations Parameter

Unit

Range

Temperature

°C °F bar psi kmole/h

5-150 41-302 1-1000 14,5-14500 10-3 - 106

Total pressure Total mass flow CO2 fugacity

bar psi mole% kmole/h Bicarbonate (HCO3-) mg/l mM Ionic strength/ salinity g/l M

7.2.3

0-10 0-145 variable variable 0-20000 0-327 0-175 0-3

Default Comments values

0

Only relevant when CO2 is given in kmole/h. The CO2 partial pressure must be < the total pressure. The allowed ranges of mole% and kmole/h CO2 are dependent on the total pressure. Default values for formation water

50

Default values for formation water

Humidity calculations

NORSOK standard

Page 10 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

Table 7.5. Input parameters for humidity calculation Parameter Temperature Total pressure Water mass flow Total mass flow

8

Unit °C °F bar psi kmole/h kmole/h

Range -16 - 200 3,2 - 392 1-1000 14,5-14500 10-3 - 106 10-3 - 106

Comments

The water mass flow must be < the total mass flow

PREDICTION OF SOME OF THE INPUT PARAMETERS

8.1 Fugacity of CO2 At high pressures gases are not ideal. To compensate for this, the partial pressure of a gas is multiplied by a fugacity constant. The real CO2 pressure can then be expressed as: fCO2 = a

.

pCO2

where: fCO2 = the fugacity of CO2 (bar) a = fugacity constant which depends on pressure and temperature pCO2 = CO2 partial pressure (bar) The CO2 partial pressure is found by one of the following expressions: pCO2 = (mole% CO2 in the gas phase/ 100% ) . P or

pCO2 = mass flow of CO2 in the gas phase (kmole/h) . P total mass flow in the gas phase (kmole/h)

where P is the total pressure in the system. The fugacity coefficient is given as /2/: a = 10

P( 0,0031 - 1,4/T)

for P < 250 bar

a = 10

250(0,0031 - 1,4/T)

for P > 250 bar

where T is the temperature in °K and P is the total pressure given in bar. The total pressure is set to 250 bar in the fugacity constant for all pressures above 250.

NORSOK standard

Page 11 of 18

CO2 corrosion rate calculation model ________________________________________________________ 8.2

pH

8.2.1

General considerations

M-506 Rev. 1, June 1998

The program contains a pH calculation module. The pH in both condensed water and formation water can be calculated. Some essential general considerations relevant for pH assessment is given below. The reported pH in water analyses is usually measured after depressurisation and atmospheric exposure of the sample. Such pH’s give no information about the in situ pH which is a requisite for the corrosion rate evaluation. The in situ pH has to be determined by calculations which take into account the three controlling buffer systems CO2 /HCO3 , H2S/HS- and CH3COOH/CH3COO-. The buffer system CH3COOH/CH3COO- can be extended to include all the other organic acids that may influence the pH determination as these acids have similar dissociation constants. The bicarbonate concentration, which is used for pH calculation, is routinely determined by titration and the reported value is set equal to the alkalinity. This is correct as long as the H2S concentration is low and the system does not contain acetic acid. For waters containing significant amount of organic acids, the reported bicarbonate concentration requires correction because organic acids contributes to the measured value of total alkalinity. The correction will be 2/3 of the organic acid concentration assuming that the end point pH of the titration is 4.3. Lower pH requires a higher fraction. More details about the interpretation of the water analysis and the determination of pH can be found in the EFC publication number 16 /3/. 8.2.2 Calculation of pH The routine for calculation of pH is based on the following chemical reactions and equilibrium constants: C CO2 (g) = CO2 (aq)

K

H

=

CO 2

p

CO 2

C CO2 (aq) + H2O = H2CO3

K = 0

H CO 2 3

C

CO 2

C

−

C

HCO

H2CO3 = H+ + HCO3-

3

K = 1

C

H CO 2 3

C

2−

C

CO

HCO3- = H+ + CO32-

+ H

3

K = 2

+ H

C

− HCO 3

NORSOK standard

Page 12 of 18

CO2 corrosion rate calculation model ________________________________________________________ H2O = H+ + OH-

=C

K

+

W H

C

M-506 Rev. 1, June 1998

− OH

The system has to be electro-neutral, which can be described by the following equation: C

+

+C + = C

Na

H

−

+ 2C

HCO

2−

+C

CO 3

−

+C −

OH

Cl

3

It is assumed that bicarbonate is added as sodium bicarbonate (NaHCO3). It is also assumed that no other salts than sodium bicarbonate and sodium chloride (NaCl) are present in the solution. These salts will dissolve as follows: NaCl = Na+ + ClNaHCO3 = Na+ + HCO3Based on these assumptions, the amount of sodium bicarbonate equals the difference in the concentrations of sodium and chloride as shown below. The mass balance for bicarbonate will therefore be as follows: C

0. Bicarb

=C

+

−C

−

Cl

Na

C0,Bicarb equals the initial amount of sodium bicarbonate. By combining the equations for the equilibrium constants with the required electro-neutrality and the mass balance for bicarbonate one get the following expression for the concentration of the Hydrogen cation: 3

C

+ H

+C

2 0 , Bicarb

C

+ H

− (K K K p H

0

+ K )C

1 CO

W

2

+ H

− 2K K K K p H

0

1

2

=0

CO 2

This equation is solved by using the Newton's Method. The pH in a condensed water system saturated with iron carbonate can also be calculated. Based on a similar deduction as above, the equation becomes:

4 2K 3 2 SP C + C + C C + + + − ( KH K0 K1 pCO + KW )C + − 2KH K0 K1 K2 pCO = 0 0, Bicarb K K K K p H H H H H 0 1 2 CO2 2 2 where KSP is the equilibrium constant of iron carbonate. 8.2.3 Equilibrium constants The equilibrium constant and the forward reaction rate constant for the carbon dioxide hydration were given by Palmer and van Eldik /4/: K0 = 0,00258

NORSOK standard

Page 13 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

The equilibrium constant for iron carbonate was taken from IUPAC /5/: KSP = 10

-(10,13 + 0,0182Tc)

molar2 where Tc is the temperature in oC.

The rest of the equilibrium constants were given by Oddo and Tomson /6/:

K

H

=

14,5 × 10 1,00258

− ( 2 ,27 + 5, 65 × 10

− ( 6,41 − 1,594 × 10

K = 387,6 × 10 1

− (10, 61− 4 ,97 × 10

K = 10 2

−3

−3

−3

T − 8,06 × 10 f

T + 8,52 × 10 f

T + 1,331 × 10 f

−6 2 T + 0,075 I ) f

molar / bar

−6 2 −5 1/ 2 + 0,1180 I ) T − 3,07 × 10 P − 0,4772 I f

−5 2 −5 1/ 2 + 0,3466 I ) T − 2 , 624 × 10 P − 1,166 I f

molar

molar

Tf : temperature given in °F. P : the pressure given in psi. I : the ionic strength given in molar. The equation for the equilibrium constant for the dissociation of water was based on data given by Delahay/7/: − ( 29 ,3868 − 0,0737549 T + 7 ,47881x10

K

w

= 10

−5 2 T )

molar

2

T: Temperature in Kelvin. 8.3 Humidity A prerequisite for corrosion to occur is that there is liquid water present in the system. In gas systems, an essential assessment is to determine if the presence of condensed water is possible. The program therefore includes a support function to calculate humidity in pure water /8/, i.e. in systems without glycol. Humidity (%) = 100 (P . FH2O)/(pH2O . Ftot) Where P = Total pressure pH2O = Water vapour pressure FH2O = Water mass flow Ftot = Total mass flow The dew point temperature (Tdew) equals the temperature where the humidity is 100%.

NORSOK standard

Page 14 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

8.4 Wall shear stress Wall shear stress is one of the parameters needed for calculation of corrosion rate. In the model, the mean wall shear stress in straight pipe sections is used. Obstacles and other geometrical changes in the flow will give rise to higher shear stresses than calculated by this program. Further, different flow regimes and geometrical obstacles may generate shear stress fluctuations where the shear stress peaks may be considerably higher than the average shear stress. High shear stress may cause mesa attacks, with corrosion rates significantly higher than what is estimated by this computer program. It is not the objective of this computer program to cover all such eventualities, and the user of the program must evaluate the flow effect in each system/part of a system based on expertise and available experience and documentation. The mean wall shear on the wall at medium to high superficial velocities of one or both of the liquid and gas velocities: S = 0,5 x ρm x f x um2

(Pa)

where the friction factor, f, can be expressed as:

f

k = 0,001375 1 + 20000 D

+ 10

6

µ

m ρ u D m m

0,33

k = Pipe roughness and D = Pipe diameter Mixture density, velocity and viscosity is expressed as: ρm = ρL λ + ρG (1 - λ) ρL = φ ρw + ρo (1 - λ) ρG = 2,7 . 14,5 . 16,018 . P . specific gravity/(Z . (460 + Tf)) φ = water cut and Z = compressibility of the gas um = uLs + uGs The liquid is considered incompressible: uLs = QL / A The gas superficial velocity is: uGs = (QG / A) Z (T/Tstd) µm = µL x λ + µG (1 - λ)

λ =

QL

QL + QG

This model /9/ is verified for medium/high flow rates by tests. If water is present the viscosity of the liquid is found as follows:

NORSOK standard

Page 15 of 18

CO2 corrosion rate calculation model ________________________________________________________

M-506 Rev. 1, June 1998

The effective viscosity of a kinetically stable oil/water mixture depends on the watercut /10/. Preferably the maximum magnitude of viscosity and the corresponding watercut should be known. The viscosity of the oil wet region, i.e. below the inversion point in a dispersed flow, can be represented as:

µ

L

=

µ

0

1

φ K

+

φ K 0

0

−

1 ,1 8 7

2 ,5

(Ns/m2 )

µo : viscosity of oil (Ns/m2 ) The value of K0 for the maximum relative viscosity µrelmax (relative to the oil) and corresponding watercut at the inversion point, φc, is equal to : K

0

φ

=

1

1 ,1 8 7

−

c

1 µ rel m ax

0 ,4

If not known, data for a medium viscosity oil/water dispersion will be used. This dispersion exhibits a maximum value of relative viscosity = 7,06 at a watercut of 0,5. The oil viscosity is equal to 0,0011 Ns/m2 at 60°C and the water viscosity is equal to 0,00046 Ns/m2. Above the inversion point, the viscosity of any dispersion is given as:

µ

L

=

µ

w

1− φ K + w 1 1− φ 1,1 8 7 − K w

2 ,5

(Ns/m2 )

µw : viscosity of water (Ns/m2 ) Where: K

w

= 1 ,1 8 7

NORSOK standard

1

φ

1

−

−

R µ rel m ax

c

0 ,4

Page 16 of 18

CO2 corrosion rate calculation model ________________________________________________________

R =

µ

M-506 Rev. 1, June 1998

water µ oil

The viscosity of water is as default given as function of temperature, Tc, given in oC /8/: 0 - 20 oC:

µ

2 1301/ ( 998,333 + 8,1855( T − 20 ) + 0,00585( T − 20 ) ) − 1,30233 c c

w

= 10

⋅ 10

−3

(Ns/m2 )

20 - 150 oC (the formula is strictly only valid up to 100 oC, but used up to 150 oC in this context): 2 (1,3272(20−T ) −0,001053(T −20) )/(T +105) c c

µ = 1002 , (10 w

−3 ) 10

(Ns/m2 )

For the medium viscosity oil at 60oC , R is equal to 0,42.

NORSOK standard

Page 17 of 18

CO2 corrosion rate calculation model ________________________________________________________

9

M-506 Rev. 1, June 1998

INFORMATIVE REFERENCES

/1/

A. Dugstad, L. Lunde, K.Videm “Parametric study of CO2 corrosion of carbon steel” NACECorrosion-94 paper No 14. /2/ C. de Waard, U. Lotz, D.E.Milliams "Predictive model for CO2 Corrosion engineering in wet natural gas pipelines", Corrosion December 1991 pp. 976 /3/ Guidelines on materials requirement for carbon and low alloy steels for H2S-containing environments in oil and gas production, European Federation of corrosion publication number 16, the Institute of Materials, 1995 /4/ D. A. Palmer and R. V. Eldik, Chem. Rev., Vol. 83, p. 651, 1983. /5/ IUPAC: Chemical Data Series No 21. Stability constants of Metal-Ion Complexes. Par A: Inorganic ligands. Pergamon Press. /6/ J. E. Oddo and M. B. Tomson, "Simplified Calculation of CaCO3 Saturation at High Temperatures and Pressures in Brine Solutions". SPE of AIME, pp. 1583, 1982. /7/ P. Delahay, “Implication of the Kinetics of Ionic Dissociation with regard to some Electrochemical Process-application to Polarography.” I.Am.Chem.Sic, 74, 1952 pp 3497. /8/ D. R. Lide, “CRC Handbook of Chemistry and Physics” 66th edition, CRC Press Inc. 19851986 /9/ A. E. Dukler, M. Wicks III, R.G. Cleveland, Frictional pressure drop in two phase flow. An approach through similarity analysis, A.I.Ch.E. Journal, Vol. 10, No 1, January 1964 /10/ H. Kvandal, T. Søntvedt, Frictional pressure loss for stable oil-water emulsions in pipeflow. Symposium on two phase flow modelling and experimentation, Rome 1995.

NORSOK standard

Page 18 of 18

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.

To keep our site running, we need your help to cover our server cost (about $400/m), a small donation will help us a lot.